ความต้านทานไฟฟ้าของธาตุ (หน้าข้อมูล)
ความต้านทานไฟฟ้า

| 0 | 1 | 2 | 3 | 4 | 5 | 6 |
| --- | --- | --- | --- | --- | --- | --- |
| T | 80 K (-193 °C) | 273 K (0 °C) | 293 K (20 °C) | 298 K (25 °C) | 300 K (27 °C) | 500 K (227 °C) |
3 Li lithium
| use | 10.0 nΩm | 85.3 nΩm | 92.8 nΩm | 94.7 nΩm | 95.5 nΩm |  |
| CRC (10-8 Ωm) | 1.00 | 8.53 | 9.28 | 9.47 | 9.55 |  |
| LNG (10-8 Ωm) |  |  | 9.28 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 9.4
4 Be beryllium
| use | 0.75 nΩm | 30.2 nΩm | 35.6 nΩm | 37.0 nΩm | 37.6 nΩm | 99 nΩm |
| CRC (10-8 Ωm) | 0.075 | 3.02 | 3.56 | 3.70 | 3.76 | 9.9 |
| LNG (10-8 Ωm) |  |  | 3.56 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 4
5 B boron
| use |  |  | 1.5×104 Ωm |  |  |  |
| LNG (10-8 Ωm) |  |  | 1.5×1012 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) > 1012
6 C carbon (diamond)
use: 
| LNG (10-8 Ωm) |  |  | 0.8 [sic] |  |  |  |
6 C carbon (graphite)
use: 
| LNG (10-8 Ωm) |  |  | 1375 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) about 1000 - direction dependent
11 Na sodium
| use | 8.0 nΩm | 43.3 nΩm | 47.7 nΩm | 48.8 nΩm | 49.3 nΩm |  |
| CRC (10-8 Ωm) | 0.80 | 4.33 | 4.77 | 4.88 | 4.93 |  |
| LNG (10-8 Ωm) |  |  | 4.77 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 4.7
12 Mg magnesium
| use | 5.57 nΩm | 40.5 nΩm | 43.9 nΩm | 44.8 nΩm | 45.1 nΩm | 78.6 nΩm |
| CRC (10-8 Ωm) | 0.557 | 4.05 | 4.39 | 4.48 | 4.51 | 7.86 |
| LNG (10-8 Ωm) |  |  | 4.39 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 4.4
13 Al aluminium
| use | 2.45 nΩm | 24.17 nΩm | 26.50 nΩm | 27.09 nΩm | 27.33 nΩm | 49.9 nΩm |
| CRC (10-8 Ωm) | 0.245 | 2.417 | 2.650 | 2.709 | 2.733 | 4.99 |
| LNG (10-8 Ωm) |  |  | 2.6548 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 2.65
14 Si silicon
use: 
| LNG (10-8 Ωm) |  |  | 105 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) about 100000
15 P phosphorus
use: 
| LNG (10-8 Ωm) |  |  | (white) 10 [sic] |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 10
16 S sulfur
| use |  |  | (amorphous) 2×1015 Ωm |  |  |  |
| LNG (10-8 Ωm) |  |  | (amorphous) 2×1023 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) > 1023
17 Cl chlorine
| use |  |  | > 10 Ωm |  |  |  |
| LNG (10-8 Ωm) |  |  | >109 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) > 1010
19 K potassium
| use | 13.4 nΩm | 64.9 nΩm | 72.0 nΩm | 73.9 nΩm | 74.7 nΩm |  |
| CRC (10-8 Ωm) | 1.34 | 6.49 | 7.20 | 7.39 | 7.47 |  |
| LNG (10-8 Ωm) |  |  | 7.2 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 7
20 Ca calcium
| use | 6.5 nΩm | 31.1 nΩm | 33.6 nΩm | 34.2 nΩm | 34.5 nΩm | 60. nΩm |
| CRC (10-8 Ωm) | 0.65 | 3.11 | 3.36 | 3.42 | 3.45 | 6.0 |
| LNG (10-8 Ωm) |  |  | 3.36 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 3.4
21 Sc scandium
use: (room temperature) (alpha, polycrystalline) calculated 562 nΩm
CRC (10-8 Ωm): (290 K-300 K) 56.2
CR2 (10-8 Ωm): (room temperature) (alpha, amorphous) 70.9
CR2 (10-8 Ωm): (room temperature) (alpha, crystalline) 26.9
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) calculated from single crystal values 56.2
| LNG (10-8 Ωm) |  |  | 56.2 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 55
22 Ti titanium
| use |  | 0.39 µΩm | 0.420 µΩm |  |  |  |
| CRC (10-8 Ωm) |  | 39 |  |  |  |  |
| LNG (10-8 Ωm) |  |  | 42.0 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 40
23 V vanadium
| use | 24.1 nΩm | 181 nΩm | 197 nΩm | 201 nΩm | 202 nΩm | 348 nΩm |
| CRC (10-8 Ωm) | 2.41 | 18.1 | 19.7 | 20.1 | 20.2 | 34.8 |
| LNG (10-8 Ωm) |  |  | 19.7 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 20
24 Cr chromium
| use |  | 118 nΩm | 125 nΩm | 126 nΩm | 127 nΩm | 201 nΩm |
| CRC (10-8 Ωm) |  | 11.8 | 12.5 | 12.6 | 12.7 | 20.1 |
| LNG (10-8 Ωm) |  |  | 12.5 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 12.7
25 Mn manganese
| use | 1.32 µΩm | 1.43 µΩm | 1.44 µΩm | 1.44 µΩm | 1.44 µΩm | 1.49 µΩm |
| CRC (10-8 Ωm) | 132 | 143 | 144 | 144 | 144 | 149 |
| LNG (10-8 Ωm) |  |  | 144 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 160
26 Fe iron
| use | 6.93 nΩm | 85.7 nΩm | 96.1 nΩm | 98.7 nΩm | 99.8 nΩm | 237 nΩm |
| CRC (10-8 Ωm) | 0.693 | 8.57 | 9.61 | 9.87 | 9.98 | 23.7 |
| LNG (10-8 Ωm) |  |  | 9.61 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 9.7
27 Co cobalt
| use |  | 56 nΩm | 62.4 nΩm |  |  |  |
| CRC (10-8 Ωm) |  | 5.6 |  |  |  |  |
| LNG (10-8 Ωm) |  |  | 6.24 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 6
28 Ni nickel
| use | 5.45 nΩm | 61.6 nΩm | 69.3 nΩm | 71.2 nΩm | 72.0 nΩm | 177 nΩm |
| CRC (10-8 Ωm) | 0.545 | 6.16 | 6.93 | 7.12 | 7.20 | 17.7 |
| LNG (10-8 Ωm) |  |  | 6.93 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 7
29 Cu copper
| use | 2.15 nΩm | 15.43 nΩm | 16.78 nΩm | 17.12 nΩm | 17.25 nΩm | 30.90 nΩm |
| CRC (10-8 Ωm) | 0.215 | 1.543 | 1.678 | 1.712 | 1.725 | 3.090 |
| LNG (10-8 Ωm) |  |  | 1.678 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 1.7
30 Zn zinc
| use | 11.5 nΩm | 54.6 nΩm | 59.0 nΩm | 60.1 nΩm | 60.6 nΩm | 108.2 nΩm |
| CRC (10-8 Ωm) | 1.15 | 5.46 | 5.90 | 6.01 | 6.06 | 10.82 |
| LNG (10-8 Ωm) |  |  | 5.9 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 5.9
31 Ga gallium
use: 
| CRC (10-8 Ωm) |  | 13.6 |  |  |  |  |
LNG (10-8 Ωm): (30 °C) 25.795
WEL (10-8 Ωm): (293 K-298 K) 14
32 Ge germanium
use: 
| LNG (10-8 Ωm) |  |  | 53000 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) about 50000
33 As arsenic
| use |  |  | 333 nΩm |  |  |  |
| LNG (10-8 Ωm) |  |  | 33.3 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 30
34 Se selenium
use: 
| LNG (10-8 Ωm) |  | (amorphous) 1.2 [sic] |  |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) high
35 Br bromine
| use |  |  | 7.8×1010 Ωm |  |  |  |
| LNG (10-8 Ωm) |  |  | 7.8×1018 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) > 1018
37 Rb rubidium
| use | 26.5 nΩm | 115 nΩm | 128 nΩm | 131 nΩm | 133 nΩm |  |
| CRC (10-8 Ωm) | 2.65 | 11.5 | 12.8 | 13.1 | 13.3 |  |
| LNG (10-8 Ωm) |  |  | 12.8 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 12
38 Sr strontium
| use | 36.4 nΩm | 123 nΩm | 132 nΩm | 134 nΩm | 135 nΩm | 222 nΩm |
| CRC (10-8 Ωm) | 3.64 | 12.3 | 13.2 | 13.4 | 13.5 | 22.2 |
| LNG (10-8 Ωm) |  |  | 13.2 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 13
39 Y yttrium
use: (room temperature) (alpha, polycrystalline) 596 nΩm
CRC (10-8 Ωm): (290 K-300 K) 59.6
CR2 (10-8 Ωm): (room temperature) (alpha, amorphous) 72.5
CR2 (10-8 Ωm): (room temperature) (alpha, crystalline) 35.5
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 59.6
| LNG (10-8 Ωm) |  |  | 59.6 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 56
40 Zr zirconium
| use | 66.4 nΩm | 388 nΩm | 421 nΩm | 429 nΩm | 433 nΩm | 765 nΩm |
| CRC (10-8 Ωm) | 6.64 | 38.8 | 42.1 | 42.9 | 43.3 | 76.5 |
| LNG (10-8 Ωm) |  |  | 42.1 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 42
41 Nb niobium
| use |  | 152 nΩm |  |  |  |  |
| CRC (10-8 Ωm) |  | 15.2 |  |  |  |  |
| LNG (10-8 Ωm) |  | 15.2 |  |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 15
42 Mo molybdenum
| use | 4.82 nΩm | 48.5 nΩm | 53.4 nΩm | 54.7 nΩm | 55.2 nΩm | 106 nΩm |
| CRC (10-8 Ωm) | 0.482 | 4.85 | 5.34 | 5.47 | 5.52 | 10.6 |
| LNG (10-8 Ωm) |  |  | 5.34 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 5
43 Tc technetium
use: 
LNG (10-8 Ωm): (100 °C) 22.6
WEL (10-8 Ωm): (293 K-298 K) 20
44 Ru ruthenium
| use |  | 71 nΩm |  |  |  |  |
| CRC (10-8 Ωm) |  | 7.1 |  |  |  |  |
| LNG (10-8 Ωm) |  | 7.1 |  |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 7.1
45 Rh rhodium
| use |  | 43.3 nΩm |  |  |  |  |
| CRC (10-8 Ωm) |  | 4.3 |  |  |  |  |
| LNG (10-8 Ωm) |  | 4.33 |  |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 4.3
46 Pd palladium
| use | 17.5 nΩm | 97.8 nΩm | 105.4 nΩm | 107.3 nΩm | 108.0 nΩm | 179.4 nΩm |
| CRC (10-8 Ωm) | 1.75 | 9.78 | 10.54 | 10.73 | 10.80 | 17.94 |
| LNG (10-8 Ωm) |  |  | 10.54 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 10
47 Ag silver
| use | 2.89 nΩm | 14.67 nΩm | 15.87 nΩm | 16.17 nΩm | 16.29 nΩm | 28.7 nΩm |
| CRC (10-8 Ωm) | 0.289 | 1.467 | 1.587 | 1.617 | 1.629 | 2.87 |
| LNG (10-8 Ωm) |  |  | 1.587 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 1.6
48 Cd cadmium
| use |  | 68 nΩm |  |  |  |  |
use: (22 °C) 72.7 nΩm
| CRC (10-8 Ωm) |  | 6.8 |  |  |  |  |
LNG (10-8 Ωm): (22 °C) 7.27
WEL (10-8 Ωm): (293 K-298 K) 7
49 In indium
| use |  | 0.080 µΩm | 83.7 nΩm |  |  |  |
| CRC (10-8 Ωm) |  | 8.0 |  |  |  |  |
| LNG (10-8 Ωm) |  |  | 8.37 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 8
50 Sn tin
| use |  | 115 nΩm |  |  |  |  |
| CRC (10-8 Ωm) |  | 11.5 |  |  |  |  |
| LNG (10-8 Ωm) |  | 11.5 |  |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 11
51 Sb antimony
| use |  | 0.39 µΩm | 417 nΩm |  |  |  |
| CRC (10-8 Ωm) |  | 39 |  |  |  |  |
| LNG (10-8 Ωm) |  |  | 41.7 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 40
52 Te tellurium
use: 
| LNG (10-8 Ωm) |  |  | (5.8-33)×103 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) about 10000
53 I iodine
| use |  | 1.3×107 Ωm |  |  |  |  |
| LNG (10-8 Ωm) |  | 1.3×1015 |  |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) > 1015
55 Cs caesium
| use | 41.6 nΩm | 187 nΩm | 205 nΩm | 208 nΩm | 210 nΩm |  |
| CRC (10-8 Ωm) | 4.16 | 18.7 | 20.5 | 20.8 | 21.0 |  |
| LNG (10-8 Ωm) |  |  | 20.5 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 20
56 Ba barium
| use | 68.3 nΩm | 302 nΩm | 332 nΩm | 0.340 µΩm | 343 nΩm | 724 nΩm |
| CRC (10-8 Ωm) | 6.83 | 30.2 | 33.2 | 34.0 | 34.3 | 72.4 |
| LNG (10-8 Ωm) |  |  | 33.2 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 35
57 La lanthanum
use: (room temperature) (alpha, polycrystalline) 615 nΩm
CRC (10-8 Ωm): (290 K-300 K) 61.5
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 61.5
| LNG (10-8 Ωm) |  |  | 61.5 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 61
58 Ce cerium (beta, hex)
use: (room temperature) (beta, polycrystalline) 828 nΩm
CRC (10-8 Ωm): (beta, hex) (290 K-300 K) 82.8
CR2 (10-8 Ωm): (room temperature) (beta, polycrystalline) 82.8
| LNG (10-8 Ωm) |  |  | (beta, hex) 82.8 |  |  |  |
58 Ce cerium (gamma, cubic)
use: (room temperature) (gamma, polycrystalline) 744 nΩm
| CRC (10-8 Ωm) |  |  |  | 74.4 |  |  |
CR2 (10-8 Ωm): (room temperature) (gamma, polycrystalline) 74.4
WEL (10-8 Ωm): (293 K-298 K) 74
59 Pr praseodymium
use: (room temperature) (alpha, polycrystalline) 0.700 µΩm
CRC (10-8 Ωm): (290 K-300 K) 70.0
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 70.0
| LNG (10-8 Ωm) |  |  | 70.0 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 70
60 Nd neodymium
use: (room temperature) (alpha, polycrystalline) 643 nΩm
CRC (10-8 Ωm): (290 K-300 K) 64.3
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 64.3
| LNG (10-8 Ωm) |  |  | 64.3 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 64
61 Pm promethium
use: (room temperature) estimated 0.75 µΩm
CRC (10-8 Ωm): (290 K-300 K) 75 est.
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 75 estimated
| LNG (10-8 Ωm) |  |  |  | 64.0 |  |  |
WEL (10-8 Ωm): (293 K-298 K) 75
62 Sm samarium
use: (room temperature) (alpha, polycrystalline) 0.940 µΩm
CRC (10-8 Ωm): (290 K-300 K) 94.0
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 94.0
| LNG (10-8 Ωm) |  |  | 94.0 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 94
63 Eu europium
use: (room temperature) (polycrystalline) 0.900 µΩm
CRC (10-8 Ωm): (290 K-300 K) 90.0
CR2 (10-8 Ωm): (room temperature) (polycrystalline) 90.0
| LNG (10-8 Ωm) |  |  | 90.0 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 90
64 Gd gadolinium
use: (room temperature) (alpha, polycrystalline) 1.310 µΩm
CRC (10-8 Ωm): (290 K-300 K) 131
CR2 (10-8 Ωm): (room temperature) (alpha, amorphous) 135.1
CR2 (10-8 Ωm): (room temperature) (alpha, crystalline) 121.7
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 131.0
| LNG (10-8 Ωm) |  |  | 131 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 130
65 Tb terbium
use: (room temperature) (alpha, polycrystalline) 1.150 µΩm
CRC (10-8 Ωm): (290 K-300 K) 115
CR2 (10-8 Ωm): (room temperature) (alpha, amorphous) 123.5
CR2 (10-8 Ωm): (room temperature) (alpha, crystalline) 101.5
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 115.0
| LNG (10-8 Ωm) |  |  | 115 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 120
66 Dy dysprosium
use: (room temperature) (alpha, polycrystalline) 926 nΩm
CRC (10-8 Ωm): (290 K-300 K) 92.6
CR2 (10-8 Ωm): (room temperature) (alpha, amorphous) 111.0
CR2 (10-8 Ωm): (room temperature) (alpha, crystalline) 76.6
CR2 (10-8 Ωm): (room temperature) (alpha, polycrystalline) 92.6
| LNG (10-8 Ωm) |  |  | 92.6 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 91
67 Ho holmium
use: (room temperature) (polycrystalline) 814 nΩm
CRC (10-8 Ωm): (290 K-300 K) 81.4
CR2 (10-8 Ωm): (room temperature) (amorphous) 101.5
CR2 (10-8 Ωm): (room temperature) (crystalline) 60.5
CR2 (10-8 Ωm): (room temperature) (polycrystalline) 81.4
| LNG (10-8 Ωm) |  |  | 81.4 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 94
68 Er erbium
use: (room temperature) (polycrystalline) 0.860 µΩm
CRC (10-8 Ωm): (290 K-300 K) 86.0
CR2 (10-8 Ωm): (room temperature) (amorphous) 94.5
CR2 (10-8 Ωm): (room temperature) (crystalline) 60.3
CR2 (10-8 Ωm): (room temperature) (polycrystalline) 86.0
| LNG (10-8 Ωm) |  |  | 86.0 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 86
69 Tm thulium
use: (room temperature) (polycrystalline) 676 nΩm
CRC (10-8 Ωm): (290 K-300 K) 67.6
CR2 (10-8 Ωm): (room temperature) (amorphous) 88.0
CR2 (10-8 Ωm): (room temperature) (crystalline) 47.2
CR2 (10-8 Ωm): (room temperature) (polycrystalline) 67.6
| LNG (10-8 Ωm) |  |  | 67.6 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 70
70 Yb ytterbium
use: (room temperature) (beta, polycrystalline) 0.250 µΩm
CRC (10-8 Ωm): (290 K-300 K) 25.0
CR2 (10-8 Ωm): (room temperature) (beta, polycrystalline) 25.0
| LNG (10-8 Ωm) |  |  | 25 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 28
71 Lu lutetium
use: (room temperature) (polycrystalline) 582 nΩm
CRC (10-8 Ωm): (290 K-300 K) 58.2
CR2 (10-8 Ωm): (room temperature) (amorphous) 76.6
CR2 (10-8 Ωm): (room temperature) (crystalline) 34.7
CR2 (10-8 Ωm): (room temperature) (polycrystalline) 58.2
| LNG (10-8 Ωm) |  |  | 58.2 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 56
72 Hf hafnium
| use | 67.5 nΩm | 304 nΩm | 331 nΩm | 337 nΩm | 0.340 µΩm | 631 nΩm |
| CRC (10-8 Ωm) | 6.75 | 30.4 | 33.1 | 33.7 | 34.0 | 63.1 |
| LNG (10-8 Ωm) |  |  | 33.1 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 30
73 Ta tantalum
| use | 26.2 nΩm | 122 nΩm | 131 nΩm | 134 nΩm | 135 nΩm | 229 nΩm |
| CRC (10-8 Ωm) | 2.62 | 12.2 | 13.1 | 13.4 | 13.5 | 22.9 |
| LNG (10-8 Ωm) |  |  | 13.5 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 13
74 W tungsten
| use | 6.06 nΩm | 48.2 nΩm | 52.8 nΩm | 53.9 nΩm | 54.4 nΩm | 103 nΩm |
| CRC (10-8 Ωm) | 0.606 | 4.82 | 5.28 | 5.39 | 5.44 | 10.3 |
| LNG (10-8 Ωm) |  |  | 5.28 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 5
75 Re rhenium
| use |  | 172 nΩm | 193 nΩm |  |  |  |
| CRC (10-8 Ωm) |  | 17.2 |  |  |  |  |
| LNG (10-8 Ωm) |  |  | 19.3 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 18
76 Os osmium
| use |  | 81.2 nΩm |  |  |  |  |
| CRC (10-8 Ωm) |  | 8.1 |  |  |  |  |
| LNG (10-8 Ωm) |  | 8.12 |  |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 8.1
77 Ir iridium
| use |  | 47 nΩm | 47.1 nΩm |  |  |  |
| CRC (10-8 Ωm) |  | 4.7 |  |  |  |  |
| LNG (10-8 Ωm) |  |  | 4.71 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 4.7
78 Pt platinum
| use | 19.22 nΩm | 96 nΩm | 105 nΩm | 107 nΩm | 108 nΩm | 183 nΩm |
| CRC (10-8 Ωm) | 1.922 | 9.6 | 10.5 | 10.7 | 10.8 | 18.3 |
| LNG (10-8 Ωm) |  |  | 10.6 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 10.6
79 Au gold
| use | 4.81 nΩm | 20.51 nΩm | 22.14 nΩm | 22.55 nΩm | 22.71 nΩm | 39.7 nΩm |
| CRC (10-8 Ωm) | 0.481 | 2.051 | 2.214 | 2.255 | 2.271 | 3.97 |
| LNG (10-8 Ωm) |  |  | 2.214 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 2.2
80 Hg mercury
| use |  |  |  | 961 nΩm |  |  |
| CRC (10-8 Ωm) |  |  |  | 96.1 |  |  |
LNG (10-8 Ωm): (solid) 21
LNG (10-8 Ωm): (liquid) 95.8
WEL (10-8 Ωm): (293 K-298 K) 96
81 Tl thallium
| use |  | 0.15 µΩm | 0.18 µΩm |  |  |  |
| CRC (10-8 Ωm) |  | 15 |  |  |  |  |
| LNG (10-8 Ωm) |  |  | 18 |  |  |  |
WEL (10-8 Ωm): (293 K-298 K) 15
82 Pb lead
| use | 49 nΩm | 192 nΩm | 208 nΩm | 211 nΩm | 213 nΩm | 383 nΩm |
| CRC (10-8 Ωm) | 4.9 | 19.2 | 20.8 | 21.1 | 21.3 | 38.3 |